 •Foreword
 •Foreword to First Edition
 •Contributors
 •Preface
 •A.1 Piezoelectric Materials
 •A.3 Optical Fiber Sensors
 •A.4 Electrorheological Fluids
 •A.5 Magnetostrictive Materials
 •A.6 MicroElectroMechanical Systems
 •A.7 Comparison Of Actuators
 •References
 •Index
 •1. Introduction and Overview
 •1.1 General
 •1.3 HighPerformance Fiber Composite Concepts
 •1.4 Fiber Reinforcements
 •1.5 Matrices
 •References
 •Bibliography
 •2. Basic Principles of Fiber Composite Materials
 •2.1 Introduction to Fiber Composite Systems
 •2.3 Micromechanics
 •2.4 Elastic Constants
 •2.5 Micromechanics Approach to Strength
 •2.6 Simple Estimate of Compressive Strength
 •References
 •3. Fibers for PolymerMatrix Composites
 •3.1 Overview
 •3.3 Carbon Fibers
 •3.4 Boron Fibers
 •3.5 Silicon Carbide
 •3.6 Aramid Fibers
 •3.7 Orientated Polyethylene Fibers
 •3.8 Dry Fiber Forms
 •References
 •4. Polymeric Matrix Materials
 •4.1 Introduction
 •4.2 Thermoset and Thermoplastic Polymer Matrix Materials
 •4.3 Thermosetting Resin Systems
 •4.4 Thermoplastic Systems
 •References
 •5. Component Form and Manufacture
 •5.1 Introduction
 •5.2 Outline of General Laminating Procedures
 •5.5 Filament Winding
 •5.7 Process Modelling
 •5.8 Tooling
 •References
 •6. Structural Analysis
 •6.1 Overview
 •6.2 Laminate Theory
 •6.3 Stress Concentration and Edge Effects
 •6.4 Failure Theories
 •6.7 Buckling
 •6.8 Summary
 •References
 •7. Mechanical Property Measurement
 •7.1 Introduction
 •7.2 Coupon Tests
 •7.3 Laboratory Simulation of Environmental Effects
 •7.4 Measurement of Residual Strength
 •7.5 Measurement of Interlaminar Fracture Energy
 •References
 •8. Properties of Composite Systems
 •8.1 Introduction
 •8.3 Boron Fiber Composite Systems
 •8.4 Aramid Fiber Composite Systems
 •8.6 Properties of Laminates
 •References
 •9. Joining of Composite Structures
 •9.1 Introduction
 •9.2 Comparison Between Mechanically Fastened and Adhesively Bonded Joints
 •9.3 Adhesively Bonded Joints
 •9.4 Mechanically Fastened Joints
 •References
 •10. Repair Technology
 •10.1 Introduction
 •10.2 Assessment of the Need to Repair
 •10.3 Classification of Types of Structure
 •10.4 Repair Requirements
 •10.6 Patch Repairs: General Considerations
 •10.7 Bonded Patch Repairs
 •10.9 Application Technology: In Situ Repairs
 •10.10 Bolted Repairs
 •References
 •11. Quality Assurance
 •11.1 Introduction
 •11.2 Quality Control
 •11.3 Cure Monitoring
 •References
 •12. Aircraft Applications and Design Issues
 •12.1 Overview
 •12.2 Applications of GlassFiber Composites
 •12.3 Current Applications
 •12.4 Design Considerations
 •12.7 A Value Engineering Approach to the Use of Composite Materials
 •12.8 Conclusion
 •References
 •13. Airworthiness Considerations For Airframe Structures
 •13.1 Overview
 •13.2 Certification of Airframe Structures
 •13.3 The Development of Design Allowables
 •13.4 Demonstration of Static Strength
 •13.5 Demonstration of Fatigue Strength
 •13.6 Demonstration of Damage Tolerance
 •13.7 Assessment of the Impact Damage Threat
 •References
 •14. ThreeDimensionally Reinforced Preforms and Composites
 •14.1 Introduction
 •14.2 Stitching
 •14.3 ZPinning
 •14.6 Knitting
 •14.8 Conclusion
 •References
 •15. Smart Structures
 •15.1 Introduction
 •15.2 Engineering Approaches
 •15.3 Selected Applications and Demonstrators
 •References
 •16. KnowledgeBased Engineering, ComputerAided Design, and Finite Element Analysis
 •16.2 Finite Element Modelling of Composite Structures
 •16.3 Finite Element Solution Process
 •16.4 Element Types
 •16.5 Finite Element Modelling of Composite Structures
 •16.6 Implementation
 •References
2
Basic Principles of Fiber Composite Materials
2.1Introduction to Fiber Composite Systems
A fiber composite material consists of a filamentary phase embedded in a continuous matrix phase. The aspect ratio (i.e., ratio of length to diameter) of the filaments may vary from about 10 to infinity (for continuous fibers). Their scale, in relation to the bulk material, may range from microscopic (e.g., 81xm diameter carbon fibers in an epoxy matrix) to gross macroscopic (e.g., 25mm diameter steel bars in concrete).
Composite constituents (fibers and matrices) can be conveniently classified according to their elastic moduli E and ductility. Within the composite, the fibers may, in general, be in the form of continuous fibers, discontinuous fibers, or whiskers (very fine single crystals with lengths of the order 1001000 ixm and diameters of the order 1  1 0 Ixm) and may be aligned to varying degrees or randomly orientated. This classification is depicted in Figure 2.1 for a number of common fibers and matrices; also listed are examples of composites formed from these materials.
2.2Mlcromechanical Versus Macromechanical View of Composites
Fiber composites can be studied from two points of view: micromechanics and macromechanics. Micromechanical analyses are aimed at providing an understanding of the behavior of composites, usually those with unidirectional fiber reinforcement, in terms of the properties of the fibers and matrices. Models of varying degrees of sophistication are used to simulate the microstructure of the composite and hence predict its properties (such as strength and stiffness) in terms of the properties and behavior of the constituents.
Macromechanics is the approach used to predict 1 the strength and stiffness of composite structures, as well as other properties such as distortion, on the basis of the "average" properties of the unidirectional material; namely, the longitudinal modulus El, transverse modulus E2, major Poisson's ratio v21 and the inplane shear modulus well as the appropriate strength values. A full analysis also
23
24 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES
= i


I 
++°+~ 
I I 
E 
L °~, 



~3 
E
O
T
I=
C 0~
I I
l+ +++
BASIC PRINCIPLES OF FIBER COMPOSITE MATERIALS 
25 
requires data on the thermal expansion coefficients of the plies in the longitudinal and transverse directions, al and a2, respectively.
Composite structural components used in aircraft are most often based on phes (sheets of unidirectional fibers or bidirectionally aligned woven fibers in a matrix) laminated together with the fibers at various orientations, as outlined in Chapter 1. Thus the properties required in the analysis are for a single ply of the composite, as described in Chapter 6. Although this analysis draws largely on data for the plies obtained from physical and mechanical testing of unidirectional composites, estimates of these properties provided by the micromechanical approach can provide useful approximate values of these properties when test data are unavailable.
2.3Micromechanics
As already mentioned, micromechanics utilizes microscopic models of composites, in which the fibers and the matrix are separately modelled. In most simple models, the fibers are assumed to be homogeneous, linearly elastic, isotropic, regularly spaced, perfectly aligned, and of uniform length. The matrix is assumed to be homogeneous, linearly elastic, and isotropic. The fiber/matrix interface is assumed to be perfect, with no voids or disbonds.
More complex models, representing more realistic situations, may include voids, disbonds, flawed fibers (including statistical variations in flaw severity), wavy fibers, nonuniform fiber dispersions, fiber length variations, and residual stresses.
Micromechanics2 can, itself, be approached in three ways:
(1)The mechanics of materials approach, which attempts to predict the behavior of simplified models of the composite material.
(2)The theory of elasticity approach, which is often aimed at producing upper and lower bound exact analytical or numerical solutions.
(3)The finiteelement (FE) approach based on t'wodimensional or threedimensional models of varying degrees of sophistication.
The most difficult aspect of the composite to model is the fiber/matrix interface, also known as the interphase, which can have a profound effect on strength and toughness. In view of this and other complexities, the FE micromechanics approach offers by far the best prospect of success to predict strength behavior. Indeed, failure theories, described in Chapter 6, require local modelling at the micromechanical level for predicting the strength of actual components.
A common aim of both approaches is to determine the elastic constants and strengths of composites in terms of their constituent properties. As previously stated, the main elastic constants for unidirectional fiber composites are:
E1 = longitudinal modulus (i.e., modulus in fiber direction)
E2 = transverse modulus
26 
COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES 


"1)12= major Poisson's ratio (i.e., ratio of contraction in the 




transverse direction consequent on an extension in the 



fiber direction) 

G 1 2 
= 
inplane shear modulus 

a l 
= 
longitudinal thermal expansion coefficient 

o¢2 = 
transverse expansion coefficient 

The main strength values required are: 


0~1 = 
longitudinal strength (both tensile and compressive) 


0u22= 
transverse strength (both tensile and compressive) 


~12 = 
shear strength 
where the superscript u refers to ultimate strength.
2.4Elastic Constants
2.4.1Mechanics of Materials Approach
The simple model used in the following analyses is a single, unidirectional ply, or lamina, as depicted in Figure 2.2. Note that the representative volume element shown, is the full thickness of the single ply and that the simplified "twodimensional" element is used in the following analyses. The key assumptions used in connection with this model are indicated in Figure 2.3.
2.4.1.1 E1 Longitudinal Modulus. The representative volume element under an applied stress is shown in Figure 2.3a. The resultant strain E is assumed to be common to both the fiber and matrix. The stresses felt by the fiber, matrix, and composite are, respectively, try,trm, and trl. Taking E/and Em as the fiber and matrix moduli, respectively, then:
Off = E f e l , Orm = E m e l , o'1 = E l e l ( 2 . 1 )
The applied stress acts over a crosssectional areaA consisting of Af, the fiber crosssection, andAm, the matrix crosssection. Because the fibers and matrix are acting in parallel to carry the load:
oqA = o'fA y ~ O'mAm or 
O"1 = 
o'f V f Jr o'm V m 
(2.2) 
where VT = AT/A = fiber volume fraction and 
Vm = A m / A = 1  
VU= matrix 

volume fraction. 



Substituting equation (2.1) into equation 
(2.2) gives: 


E1 = EfVf + EmVm 
(2.3) 
Equation (2.3) is a "ruleofmixtures" type of relationship that relates the composite property to the weighted sum of the constituent properties.
BASIC PRINCIPLES OF FIBER COMPOSITE MATERIALS 
27 

T 



, ... j/ T 

Model 

, 
_L thickness t 



Volum e 
J_ 
element 
1 

thickness t 

T 

2 
~ !
Simplified 

2D element 
...... Matri x 

F///~ .~o~~ ' / / ~ 

Matrix 
Fig. 2.2 Model and representative volume element of a unidirectional ply.
Experimental verification of equation (2.3) has been obtained for many fiber/ resin systems; examples of the variation of El with Vf for two glass/polyester resin systems are shown in Figure 2.4.
2.4.1.2 E2 Transverse Modulus. As shown in Figure 2.3b, the fiber and matrix are assumed to act in series, both carrying the same applied stress o.2. The transverse strains for the fiber, matrix, and composite are thus, respectively:

o.2 
o2 
= 
o.2 
(2.4) 
> 8f 
= ~ 
' 8m ~ g m ' 82 
  



E2 

where E} is the effective transverse modulus of the fiber.
28 
C O M P O S I T E MATERIAL S FO R A I R C R A F T S T R U C T U R E S 



Undeformed 



element 




=I 

T ~ / ~ 
Matrix 
 

_ L I 
.Fi.ber / / / ~ 1 


Matrix 
I 


I_ 
L 
I 

i 
I 


Applied stresses 
Deformations 
Relationship 



E= = E f V f + E m (1Vf) 
a. 
Determination of E1 

HaLl 






l l l l t l l 
F.... . ].Law 
l/E= = v f / E f + ( 1  V f ) / E m 



b///////~ s 



i l l 111~ o, 
Ii 
il 






b. 
Determination of E= 






Z~WIZ 
ul==hVf+U m (1Vf) 

Determination of ul= 




 T 


1/G1= = Vf/Gf + (1  Vf) / Gm 





IJJJJJJJA,l 
/ t . f ~ 
AmlZ 

Determination of G~z
Fig. 2.3 Models for the determination of elastic constants by the "mechanics of materials" approach.
BASIC PRINCIPLES OF FIBER COMPOSITE MATERIALS 
29 
60
~d
50
0
40
0
0
O.. 30 t.~
20
10 








¢ 1 








¢ 








0 
I 
I 
I 
I 
I 
I 
I 
I 
0 
0.1 
0.2 
0.3 
0.4 
0.5 
0.6 
0.7 
0.8 
Vf
Fig. 2.4 E1 versu s fiber volume fraction Vf for two glass/polyester systems.
Deformations are additive over the width W, so that:
a W 
= a W ~ + a W m 


or 




82W = 
~,f(Wf W ) "] ,~m(VmW ) 
( 2 . 5 ) 

Substitution of equation (2.4) into equation (2.5) yields: 



1 _ 
Vf 
~ Vm 
(2.6) 
E2 
E~ 
Em 

Experimental results are in reasonable agreement with equation (2.6) as shown, for example, in Figure 2.5, for a glass/polyester composite.
30 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES
20 
I
I
I
#
I
15
10
5
I I I I I
t 
i 
i 
0 
0.1 
0.2 
0.3 
0.4 
0.5 
0.6 
0.7 
0.8 
V~
Fig. 2.5 E2 versus Vffor two glass/polyester systems, solid lines are based on Eq. 2.6.
In contrast to glass fibers, which are isotropic, with an Ef around 72 GPa, carbon fibers are highly anisotropic (stiffness varies with direction), having Ef around 200 GPa and E) around 7 GPa.
Several interesting features emerge from equations (2.3) and (2.6). In highperformance composites, the fiber moduli are much greater than the resin moduli, so that, in the typical fiber/volume fraction range of 5 0  6 0 % , the matrix has only a small effect upon E1 while the fibers have only a small effect on E2. In other words,
~ E m
E1 "~ EfVf, E2 ~   Vm
BASIC PRINCIPLES OF FIBER COMPOSITE MATERIALS 
31 
2.4.1.3 Major Poisson's Ratio v12. The major Poisson'sratio is defined by:
Y12 = 
82 
(2.7) 
    


81 

where the only applied stress is o"1 (Fig. 
2.3c). 

The transverse deformation is given by
~ W = ,SWz + hWm
o r
e 2 W =  1 ) f e l ( V f W )  llmSl(Vm W ) 
(2.8) 
Substituting for e2 from equation (2.7) into equation (2.8) gives the result
va2 = vfVf + vmVm 
(2.9) 
which is another ruleofmixtures expression.
2.4. 1.4 G12 InPlane Shear Modulus. The applied shear stresses and resultant deformations of the representative volume element are shown in Figure 2.3d. The shear stresses felt by the fiber and matrix are assumed to be equal, and the composite is assumed to behave linearly in shear (which is, in fact, not true for many systems).
The total shear deformation is given by:
A = yW
where y is the shear strain of the composite. The deformation A consists of two additive components, so that:
y W = yf(YfW) 1 "~m(VmW) 
(2.10) 
Because equal shear stresses are assumed:
T 
T 


"~f "~ G f f , 
"~m = ~ m ' 
"~ : , / V 1 2 
(2.11) 
substitution of equation (2.11) into equation (2.10) yields:
1 _ Vf ~ Vm 
(2.12) 
G12 Gf Gm
Because Gm is much smaller than Gf, the value of Grnhas the major effect on G12 for typical 5 0  6 0 % Vf values; the situation is analogous to that for the transverse modulus E2.
32 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES
2.4.2 Refinements to Mechanics of Materials Approach for E1 and E2
2 . 4 . 2 . I Predictio n o f El. Equation (2.3) is considered to provide a good estimate of the longitudinal modulus E1; however it does not allow for the triaxial stress condition in the matrix resulting from the constraint caused by the fibers. Ekvall3 has produced a modified version of the equation to allow for this effect
E1 = E:V f + E'~Vm 
(2.13) 
where
E~
E~ (1  2v2~)
and vm is Poisson's ratio for the matrix material. However, the modification is not large for values of Vm of approximately 0.3.
2.4.2.2 Prediction of E2. Equation (2.6) is considered to provide only an approximate estimate of the transverse modulus E2. This is because, for loading in the transverse direction, biaxial effects resulting from differences in contraction in the longitudinal (fiber) direction between the fiber and the matrix become significant. The contraction difference arises because the two phases experience different strains, and this is even more marked if there is a difference in their Poisson's ratios.
The modified version of equation (2.6) produced by Ekvall3 is
1 
V: ~ V m 
Vf [(Efvm//Em) 1if]2 
  
Ef Em 
( 2 . 1 4 ) 
E2 
Ef [(VfEf/VmEm) 'FI] 
2.4.3Theory of Elasticity Approach to the Elastic Constants
The theory of elasticity approach to the determination of the elastic constants for composites is based on a wide variety of models and energy balance treatments. A detailed discussion of these approaches is beyond the scope of this chapter; however, some aspects are outlined here.
2.4.3. I Energy Approach. Bounding (or variational) derivations use energy balance considerations to produce upper and lower bounds on the elastic constants. The usefulness of the results, of course, depends upon the closeness of the bounds, as demonstrated in the following example.
Considering the stressed element shown in Figure 2.3a, it can be shown4 that the lower bound on the longitudinal modulus E1 is given by:
1 < Vm V: 
( 2 . 1 5 ) 
BASIC PI.IINCIP'Lk::S UIPIBPH L;OMPUS I I ~ MA I ~HIAL S
Compare with equation (2.6), while the upper bound is given by:
1  
vf   4V/1'12 I 2V22 

E1 < 
1  v f 
E f Vf 
 
 2 v } 

+ 1   V m   4 V m V l 2 + 2 p 2 2 E m V m 


1  
Vm  2V2 
where
( l   P m   
2 
2 V m ) ' P f E f V f Jr (1  vf  2 1 ) ~ ) v m E m V m 

1)12   
 2 v 2 ) E f V f + (1  v f  2 l ) } ) E m V m 
(1  v,, 
33
(2.16)
It is o f interest to note that if vie = vf = Vm, the upper bound solution becomes:
El <_EfVf + EmVm
which is the same result as equation (2.3),which implies an equalityof vfand Vm in the mechanics of materials approach.
In this example,the bounding solutionsare not very usefulbecausethe bounds are too far apart, the lower bound being the transverse modulus as predicted by the mechanics of materials approach.
2 . 4 . 3 . 2 D i r e c t A p p r o a c h e s . Here, various representative models o f elastic inclusions in an elastic matrix are employed to obtain exact solutions for the stiffness properties. Typical volume elements assumed for a hexagonal and a square fiber distribution are shown in Figure 2.6. In m a n y cases, the solutions are highly complex and o f limited practical use. Regular fiber distributions do not occur in practical composites. Rather, the array is random and the analysis for regular arrays must be modified to allow for the extent o f contact between fibers. This is called the degree o f contiguity 5 and is measured b y a coefficient c, which can vary from c = 0 for isolated fibers to c = 1 for contacting fibers. This
situation is illustrated in Figure 2.7. The effective value o f c 
ma y be determined 

experimentally. The degree o f contiguity has more effect o n 
E 2 and G12 than on 

E 1. These 
matters, and other simplifying approaches, such 
as the HalpinTsai 
equations, 
are discussed more fully in Ref. 5. 

2.4.4Expansion Constants c~1and OZ2
The coefficients o f thermal expansion o~1 and a2 for the unidirectional ply are required, for example, in the thermomechanical analysis o f multidirectional laminates.
The actual values o f the two constants derive from the expansion coefficients o f the fibers a f and matrix am, and their orientation. Differences between a f and
34 COMPOSITE MATERIALS FOR AIRCRAFT STRUCTURES
" ~ 
SIMPLIFIED 

REPRESENI'ATIVE 

VOLUME ELEMENT 
REPRESENTATIVE 

VOLUME 
ELEMENT 
Hexagonalarray and representative volume elements, 
< )(D( >

r  r   1 
O 
J 

Z 
>'G'{) 


SIMPLIFIED 

I._J._ J 


( )d)E) 

REPRESENTATIVE 


VOLUME ELEMENT 

REPRESENTATIVE 

VOLUME ELEMENT
Fig. 2.6 Typical models of composites for exact elasticity solutions.
OLm give rise to internal stresses and possibly distortion when coolin g laminates after manufacture and during subsequent service.
2.4.4. I Longitudinal Expansion Coefficient o~1. A simple estimate of el can be mad e based on the model in Figure 2.3 used to estimate E 1. W e have that:


O ' f 
O"m 

,Z.1 = e f = 
P'm = ~ff ~ a f A T = Em + ° l m A T 

where AT = 
temperature change. 


Also, since there are no external stresses: 




o ) VI = O'm(]  
VD 
This leads to: 





EfotfVf + Emo~m(1  VT) 


OZ1 
= 
(2.17) 


Ef Vf + Era(1 
 Vf) 
Because, in 
man y composites, a f << am the 
c~f term can be ignored in the 

equation. 



2.4.4.2 Transverse Expansion Coefficient oL2. A simple ruleofmixtures estimate o f c~2 is obtained assuming the series model used in Figure 2.3. To
BASIC PRINCIPLES OF FIBER COMPOSITE MATERIALS 
35 
0 0 0
0 0 0
C=O 
C1 
ISOLATED FIBERS 
ISOLATED MATRIX 
RESIN CONTIGUOUS 
FIBERS CONTIGUOUS 
Extremes of fiber contiguity.
Schematic diagram of actual fiber arrangement
Fig. 2.7 Concept of contiguity used for semiempiricalelasticity solutions.
e s t i m a t e E 2 we have that
a2 = a } v l + am(1  Vl) 
(2.18) 
where a} is the transverse expansion coefficient for the fiber, which often differs significantly from the longitudinal value aT. Carbon fibers represent an extreme
case o f variation because 
the fiber 
is highly anisotropic. 
Thus, although 
ae is 

around 0, the a} is around 
l 0 
60 
C 
1 
• 
am 
55 x l 0 
60   1 



. For the epoxy resin 

C 
However, this model does not account for any interaction between the fiber and matrix, due in part to ignoring differences in Poisson's ratio, and leads to the conclusion that there are no thermally induced stresses between the fiber and matrix.
I f interaction is included, it can be shown z that: 


a2 
= a'fVf + am(1  Vf) + (E~vm  
E,nvm~ 
(2.19) 


\ " 
El 
 ) ( a m  a f ) ( 1  V f ) V f 

Тут вы можете оставить комментарий к выбранному абзацу или сообщить об ошибке.
Оставленные комментарии видны всем.